Presentation on theme: "FAA William J. Hughes Technical Center Probability of Detection Studies to Quantify Flaw Detection in Composite Laminate Structures Probability of Detection."— Presentation transcript:
FAA William J. Hughes Technical Center Probability of Detection Studies to Quantify Flaw Detection in Composite Laminate Structures Probability of Detection Studies to Quantify Flaw Detection in Composite Laminate Structures Sandia is a multiprogram laboratory operated by Sandia Corporation, a Lockheed Martin Company, for the United States Department of Energys National Nuclear Security Administration under contract DE-AC04-94AL85000. Dennis Roach & Tom Rice Sandia National Labs FAA Airworthiness Assurance Center A340 HTP Skin
FAA William J. Hughes Technical Center ITG Team Participants Inspection Task Group Team Participants CACRC Inspection Task Group Members: Wolfgang Bisle – Airbus Chris Dragan – Polish Air Force Institute of Technology Don Duncan – US Airways Jim Hofer – Boeing Quincy Howard – Boeing Jeff Kollgaard – Boeing Francois Landry – Bell Helicopter Robert Luiten – KLM Airlines Alex Melton – Delta Air Airlines Eric Mitchell – American Airlines Stephen Neidigk – Sandia Labs AANC Keith Phillips – Airbus Tom Rice – Sandia Labs AANC Dennis Roach – Sandia Labs AANC (Chair) Vilmar da Silva do Vale – Embraer Dennis von Seelen - Lufthansa Technik Darrell Thornton – UPS Sam Tucker – United Airlines Roy Wong – Bombardier Rusty Jones, Larry Ilcewicz, Dave Galella, Paul Swindell – FAA
FAA William J. Hughes Technical Center Composite Structures on Boeing 787 Aircraft Carbon laminate Carbon sandwich Fiberglass Aluminum Aluminum/steel/titanium pylons A380 Pressure Bulkhead Composite Center Wing Box Program Motivation - Extensive/increasing use of composites on commercial aircraft and increasing use of NDI to inspect them Program Goals: Assess & Improve Flaw Detection Performance in Composite Aircraft Structure
FAA William J. Hughes Technical Center One airline reports 8 composite damage events per aircraft (on avg.) with 87% from impact; cost = $200K/aircraft Sources of Damage in Composite Structure Bird Strike Towing Damage Lightning Strike on Thrust Reverser Disbonding at skin-to- honeycomb interface
FAA William J. Hughes Technical Center Significant Internal Damage Source: Carlos Bloom (Lufthansa) & S. Waite (EASA) Inspection Challenge – Hidden Impact Damage Backside fiber failure from ice impact Visible Impact Damage – external skin fracture Backside Damage – internal skin fracture & core crush Extent of Visible Damage from Outside Damage from ground vehicle
FAA William J. Hughes Technical Center Experiment to Assess Flaw Detection Performance Composite Flaw Detection Experiment Participation from over 25 airlines and maintenance depots Industry-wide performance curves generated to quantify: How well current inspection techniques are able to reliably find flaws in composite honeycomb structure The degree of improvements possible through integrating more advanced NDI techniques and procedures. Composite Honeycomb Flaw Detection Experiment Blind application of techniques to study hits, misses, false calls, and flaw sizing
FAA William J. Hughes Technical Center Purpose Determine in-service flaw detection capabilities: 1) conventional NDT methods vs. 2) improvements through use of advanced NDT. Optimize laminate inspection procedures. Compare results from hand-held devices with results from scanning systems (focus on A-scan vs. C-scan and human factors issues in large area coverage). Provide additional information on laminate inspections for the Composite Repair NDT/NDI Handbook (ARP 5089). An Experiment to Assess Flaw Detection Performance in Composite Laminate Structures 737 Composite Horiz. Stabilizer A380 Fuselage Section 19
FAA William J. Hughes Technical Center Approach Statistical design of flaws and other variables affecting NDI - range of types, sizes & depths of flaws Study factors influencing inspections including composite materials, flaw profiles, substructures, complex shapes, fasteners, secondary bonds, and environmental conditions POD and signal-to-noise data gathering NDI Ref. Stds. prepared to aid experiment Flaw Detection in Solid Laminate Composites Expected Results - evaluate performance attributes 1) accuracy & sensitivity (hits, misses, false calls, sizing) 2) versatility, portability, complexity, inspection time (human factors) 3) produce guideline documents to improve inspections 4) introduce advanced NDI where warranted
FAA William J. Hughes Technical Center Specimen Types – Solid laminate carbon (12 to 64 plies) Contoured and tapered surfaces Substructures – stringers, ribs, spars; honeycomb impediment Bonded & sealed joints; fasteners Large enough to warrant scanners; complex geometry to challenge scanners Carbon, uniaxial tape Specimen Design - Flaw Detection in Solid Laminate Composites Flaw Types - statistically relevant flaw distribution with range of sizes & depths (near front & back surfaces; in taper regions) 1) interply delaminations (kissing and air gap) 2) substructure damage 3) skin-to-stiffener disbonds 4) simulated impact damage
FAA William J. Hughes Technical Center Thick Laminate With Complex Taper - Fabrication Flaw templates - ensure proper location of flaws Flaws inserted
FAA William J. Hughes Technical Center Thick Laminate With Complex Taper - Fabrication
FAA William J. Hughes Technical Center Thick Laminate With Complex Taper Type I Specimen
FAA William J. Hughes Technical Center 20 Ply Ref Std 32 Ply Ref Std Reference Standards – Feedback Panels
FAA William J. Hughes Technical Center Specimen Set - Flaw Detection in Solid Laminate Composites Thickness Range: 12 – 64 plies Inspection Area: 46 ft. 2 Number of Flaws: 202
FAA William J. Hughes Technical Center Specimen Set - Flaw Detection in Solid Laminate Composites Thickness Range: 12 – 64 plies Simple Tapers Complex tapers Substructure Flaws Curved Surfaces Array of flaw types NDI Ref. Stds.
FAA William J. Hughes Technical Center Solid Laminate Experiment Participants
FAA William J. Hughes Technical Center Solid Laminate Flaw Detection Experiment Implementation PODs calculated for overall laminate, by thickness family, by substructure effects, by complex geometry effects, by flaw types, etc. 57 inspectors
FAA William J. Hughes Technical Center POD Curves for 12-20 Ply Solid Laminate Family False Calls: Constant thickness = 0.4/inspector Complex Geometry = 4.0/inspector 34 ft. 2 inspection area Individual and Cumulative Comparisons Flaw Size (Diameter in Inches) Probability of Detection Overall: POD [90/95] = 1.29 dia. Constant Thickness (12, 20, 28 plies): POD [90/95] = 0.86 dia. Complex Geometry (tapered, curved, substructure, fasteners, honeycomb): POD [90/95] = 1.49 dia.
FAA William J. Hughes Technical Center POD Improvements from Use of Methods to Ensure Proper Coverage Flaw Size (Diameter in Inches) Probability of Detection
FAA William J. Hughes Technical Center POD Curves for 20-32 Ply Solid Laminate Family False Calls: Constant thickness = 0.8/inspector Complex Geometry = 0.3/inspector 12 ft. 2 inspection area Overall: POD [90/95] = 0.82 dia. Constant Thickness (32 plies): POD [90/95] = 0.74 dia. Complex Geometry (tapered, curved, substructure, fasteners, honeycomb): POD [90/95] = 0.93 dia. Substructure: POD [90/95] = 1.50 dia. Individual and Cumulative Comparisons Flaw Size (Diameter in Inches) Probability of Detection
FAA William J. Hughes Technical Center Desire to Transition Inspectors from Average to Good to Outstanding Flaw Size (Diameter in Inches) Probability of Detection
FAA William J. Hughes Technical Center Overall Performance of Pulse-Echo UT for Flaw Detection in Composite Laminates Overall Performance of Pulse-Echo UT for Flaw Detection in Composite Laminates Flaw Size (Diameter in Inches) Probability of Detection Overall: POD [90/95] = 1.13 dia. Constant Thickness (32 plies): POD [90/95] = 0.80 dia. Complex Geometry (tapered, curved, substructure, fasteners, honeycomb): POD [90/95] = 1.33 dia.
FAA William J. Hughes Technical Center Ramp Damage Check Experiment (RDCE) – Spin Off Subset of Solid Laminate Experiment Purpose: to assess new, ultrasonic-based Go/No-Go equipment that OEMs plan to deploy at airports and other non-scheduled maintenance depots using non-NDI personnel (e.g. A&Ps). Usage Scenario: the equipment will be deployed whenever visual clues or other events occur which warrant closer scrutiny of a composite laminate structure; ground personnel, with appropriate training on such equipment, will set up the equipment in accordance with OEM-supplied procedures, and then make an assessment of the region in question. Limitations: such Go/No-Go UT equipment is intended to be used to assess local indications or regions only, not for wide-area inspections; equipment operators are directed to very distinct locations.
FAA William J. Hughes Technical Center Ramp Damage Check Experiment – Ultrasonic Devices with Go/No-Go Capabilities Olympus – Ramp Damage Checker General Electric – Bondtracer
FAA William J. Hughes Technical Center Ramp Damage Check Experiment – POD Curves for Composite Laminates Flaw Size (Diameter in Inches) Probability of Detection Overall: POD [90/95] = 0.78 dia. Similar results for GE Bondtracer and Olympus Ramp Damage Checker Similar performance from both inspectors and A&P mechanics Less spray in individual performances False Calls = 0.6/inspector 14 ft. 2 inspection area
FAA William J. Hughes Technical Center Thermography MAUS System SAM System Shearography Wide Area and C-Scan Inspection Methods PE Phased Array UT UT Wheel Array UltraImage Scanner
FAA William J. Hughes Technical Center Solid Laminate Experiment – Advanced NDI Testing Evaluations Solid Laminate Experiment – Advanced NDI Testing Evaluations Pulsed Thermography – Thermal Wave Imaging Phased Array UT – Olympus Omniscan Phased Array UT – Toshiba Matrix Eye Phased Array UT – Sonatest RapidScan Phased Array UT – Boeing MAUS V Phased Array UT – GE RotoArray & Phasor Microwave – Evisive Digital Acoustic Video – Imperium Acoustocam Ultrasonic Video - DolphiCam Line Infrared – Mistras Shearography – LTI Shearography – Dantec Backscatter X-ray – Scannex Acousto Ultrasonics – Physical Acoustic Corp. T-SCOUT Locked-In Infrared – MovieTherm Laser UT – iPhoton
FAA William J. Hughes Technical Center Sample of POD Results for Composite Flaw Detection Performance of Advanced NDI Flaw Size (Diameter in Inches) Probability of Detection
FAA William J. Hughes Technical Center Survey of Industry Composite NDI Training Only 25% of responders currently have special composite NDI training in place
FAA William J. Hughes Technical Center Question 5 – Do inspectors also receive general composite training to understand composite materials, plies, lay-ups, scarfed repairs, composite design, composite processing, etc.? Question 15 - If experience level is a factor in determining qualification to perform certain inspections, do you use some sort of apprentice program to expose newer inspectors to such inspections?
FAA William J. Hughes Technical Center Results can be used by OEMs and airlines to: 1) define detectability for various flaws/damage, 2) guide NDI deployment & training; used by FAA to produce guidance documents. Flaw Detection - Conventional, manually-deployed PE-UT: POD [90/95] = 1.12 dia.; skin flaw detection is higher, flaw detection in substructure is more challenging (POD [90/95] = 1.34 dia.) False Call rates were extremely low: 1 false call per 17 ft. 2 (flaws 0.25 in. 2 ) Optimum inspection rates = 2 ft. 2 /hour NDI Performance Obstacles – attenuation, complex signal reflections, confounding presence of signal harmonics, rapid variations produced by changing/complex geometry, optimum deployment and difficulty with inspecting large areas Controlled and Proper Use of Ramp Damage Check Go/No-Go equipment can produce good performance (POD [90/95] = 0.77 dia.) Caution – proper calibration area must be used; requires good schematics (available?) Cannot be used in taper or changing geometry regions Conclusions – Inspection of Solid Laminate Structures
FAA William J. Hughes Technical Center Recommendations – How to move inspections from average to good to outstanding Increased exposure to representative composite inspections – common industry NDI Feedback Specimens Increased, focused composite NDI training (ARP covering 1 st two bullets) Use of NDI and composite shop apprenticeships (OJT, awareness training, formal/uniform use of this tool) Enhanced NDI procedures – deployment, signal interpretation, clearer schematics showing structural configuration Use of inspection coverage aids should be required Divide large area inspections into a number of smaller regions Add audible alarms & detection lights to probe in Go/No-Go devices Prepare additional industry guidance to address training, use of NDI Reference and Proficiency specimens, procedures, composite construction awareness – produced by joint effort of OEMs, Airlines, FAA & industry groups
FAA William J. Hughes Technical Center 2013 Airlines for America NDT Forum POD Studies to Quantify Flaw Detection in Composite Laminate Structures Dennis Roach Tom Rice FAA Airworthiness Assurance Center Sandia National Laboratories Composites have many advantages for use as aircraft structural materials including their high specific strength and stiffness, resistance to damage by fatigue loading and resistance to corrosion. The aircraft industry continues to increase its use of composite materials, most noteworthy in the arena of principle structural elements. This expanded use, coupled with difficulties associated with damage tolerance analysis of composites, has placed greater emphasis on the application of accurate nondestructive inspection (NDI) methods. Traditionally, a few ultrasonic-based inspection methods have been used to inspect solid laminate structures. Recent developments in more advanced NDI techniques have produced a number of new inspection options. Many of these methods can be categorized as wide area techniques that produce two- dimensional flaw maps of the structure. An experiment was developed to assess the ability of both conventional and advanced NDI techniques to detect voids, disbonds, delaminations, and impact damage in adhesively bonded composite aircraft structures. A series of solid laminate, carbon composite specimens with statistically relevant flaw profiles were inspected using conventional, hand-held pulse echo UT and resonance, as well as, new NDI methods that have recently been introduced to improve sensitivity and repeatability of inspections. The primary factors affecting flaw detection in laminates were included in this study: material type, flaw profiles, presence of complex geometries like taper and substructure elements, presence of fasteners, secondarily bonded joints, and environmental conditions. This experiment utilized airline personnel to study Probability of Detection (POD) in the field and to formulate improvements to existing inspection techniques. In addition, advanced NDI methods for laminate inspections – such as thermography, shearography, scanning pulse-echo UT, ultrasonic spectroscopy, laminography, microwave and phased array UT – were applied to quantify the improvements achievable through the use of more sophisticated NDI. This paper presents the experiment design used to evaluate applicable inspection techniques and the key results from the POD testing conducted at multiple airline facilities.